# applied origami using origami design principles to fold ... applied origami using origami design...

Post on 18-Jan-2020

85 views

Embed Size (px)

TRANSCRIPT

APPLIED ORIGAMI

Using origami design principles to fold reprogrammable mechanical metamaterials Jesse L. Silverberg,1* Arthur A. Evans,2 Lauren McLeod,1 Ryan C. Hayward,3

Thomas Hull,4 Christian D. Santangelo,2 Itai Cohen1

Although broadly admired for its aesthetic qualities, the art of origami is now being recognized also as a framework for mechanical metamaterial design. Working with the Miura-ori tessellation, we find that each unit cell of this crease pattern is mechanically bistable, and by switching between states, the compressive modulus of the overall structure can be rationally and reversibly tuned. By virtue of their interactions, these mechanically stable lattice defects also lead to emergent crystallographic structures such as vacancies, dislocations, and grain boundaries. Each of these structures comes from an arrangement of reversible folds, highlighting a connection between mechanical metamaterials and programmable matter. Given origami’s scale-free geometric character, this framework for metamaterial design can be directly transferred to milli-, micro-, and nanometer-size systems.

M etamaterials are rapidly emerging at the frontier of scientific and technological in- novation due to their exotic and tunable material properties, which arise from ar- rangements of smaller units within the

bulk system (1–5). Once fabricated, structural mod- ifications are generally difficult, making it rare to find metamaterials that can be reconfigured beyond their original design. Origami-inspired mechanical metamaterials offer enhanced flex- ibility in performance because their properties are coupled to a dynamically alterable folding pat- tern (6–16). Hence, multiple stable configurations can manifest from a single structure yielding pro- grammable metamaterials. We studied the Miura-ori tessellated folding

pattern, which has recently been proposed as an origamimetamaterial (Fig. 1, A to C, figs. S1 to S3, and movie S1) (14, 15). Historically, this design was invented to efficiently pack solar panels for spacemissions (17), but the morphology also nat- urally occurs in leaves (18) and embryonic in- testine (19, 20) and generally arises when thin sheets tethered to a surface undergo biaxial com- pression. The geometry of aMiura-ori is a herring- bone pattern that emerges from a series of convex mountain and concave valley creases (Fig. 1C). Vertices are formedwhen four creases intersect, and four adjacent vertices bound equal-area facets arranged with inversion symmetry (Fig. 1B). This fold pattern defines a lattice characterized by two static crease lengths ‘1; ‘2, and one static plane angle a. To quantify folding, a vertex angle e is

required (Fig. 1C); when e = 180° – 2a, the structure is maximally contracted into a folded state, and when e = 180°, the structure is an unfolded flat sheet. If folded from an ideal material with infinite

stretching modulus, the Miura-ori would have only one degree of freedom described by e (14). However, generating samples from laser-cut sheets of paper and mylar (Fig. 1C) (see supplementary materials for details), we find additional degrees of freedom, as evidenced by soft bending modes (14, 15). As an extreme example, the Miura-ori supports highly localized heterogeneity intro- duced after folding by applying force to a vertex in the normal direction and popping it into a categorically different mechanically stable state (Fig. 2A, fig. S4A, and movie S2). This pop- through defect (PTD) changes lattice topology by suppressing one fold and bending adjacent facets through an angle f (Fig. 2, B and C). Quantify- ing lattice distortion by the surface’s Monge patch mean curvature calculated from three- dimensional (3D) digitized scans, we find that displacements of vertices in the xy plane are negligible within a distance of one unit cell; this compares favorably with theoretical pre- dictions that estimate a distortion decay length ≈1/2 the unit cell width (Fig. 2D) (see supplemen- tarymaterials for details) (21, 22). Although highly localized, PTDs are unlike conventional lattice defects because they involve only elastic facet bending and hence are reversibly removable. To determine the robustness of PTDs tomechan-

ical perturbations, we theoretically model a single unit cell with one mountain and three valley folds in mechanical equilibrium (similar to the paper model in Fig. 2, B and C). To account for experimentally observed facet bending, two ad- ditional symmetrically placed creases are included whose folding angles f are equal and have equi- librium values of 180° (14, 15). We assume a

Hookean energy expression for all creases and calculate the dimensionless energy u as a func- tion of the folding configuration (Fig. 2E and fig. S5) (see supplementary materials for details). We observe that the energy landscape has two distinct regions, each with its own local min- imum (Fig. 2E, points I and II), that are con- nected at a single point corresponding to a fully unfolded unit cell where f = e = 180°. For mate- rials with a finite stretching modulus, this con- necting point widens along the f axis and allows for otherwise forbidden stretching-enabled tran- sitions. Because the stretching modulus is pro- portional to sheet thickness (23), the energy required to transition between states is a tunable design feature. Thus, while PTDs are introduced reversibly, their stability to mechanical perturba- tions is controlled by the competition between the material’s bending and stretching energy scales. The mechanical consequences of a PTD were

determined by folding laser-cut structures from 24-lb paper with s2 unit cells, where swas varied from 3 to 8 and a was fixed at 60°. A centrally located defect was introduced by hand, and the compressive modulus Kdefecty ðeÞ was measured as a function of defect density n = 1/s2 (see sup- plementary materials for details). Normalizing these data by the modulus of a defect-free lattice, Knormaly ðeÞ, revealed a divergence in stiffness as a function of compression limited only by tearing of the sheet at the highest strains (Fig. 2F and fig. S4B). This divergence arises from a violation of Maekawa’s theorem, which requires the number of mountain folds minus the number of valley folds at every vertex to be T2 for a structure to fold flat (24). By linking enhanced mechanical stiffness to violations of a canonical paper- folding theorem, these data experimentally demon- strate how geometric constraints in origami-based design can dominate bulk material properties.

SCIENCE sciencemag.org 8 AUGUST 2014 • VOL 345 ISSUE 6197 647

1Physics Department, Cornell University, Ithaca, NY 14853, USA. 2Department of Physics, University of Massachusetts, Amherst, MA 01003, USA. 3Department of Polymer Science and Engineering, University of Massachusetts, Amherst, MA 01003, USA. 4Department of Mathematics, Western New England University, Springfield, MA 01119, USA. *Corresponding author. E-mail: JLS533@cornell.edu

Fig. 1. Schematic and 3D reconstruction of the Miura-ori with definition of important geometric parameters. (A) TheMiura-ori crease pattern on a flat sheet is depicted with alternating mountain (red) and valley (blue) folds. (B) Each facet is bounded by four vertices labeled 1 through 4. (C) An experimentally recorded 3D image of a 4 by 4 laser-cut Miura-ori with two in-plane projections shows the folded structure at equilibrium. The color bar gives height in mm.

RESEARCH | REPORTS

o n

D ec

em be

r 8,

2 01

6 ht

tp ://

sc ie

nc e.

sc ie

nc em

ag .o

rg /

D ow

nl oa

de d

fr om

http://science.sciencemag.org/

Nevertheless, such constraints are stillmalleable; the value of e where Kdefecty increases is shifted simply by varying n. Thus, PTDs make attractive elements for metamaterial design because the on- set and strength of Kdefecty are rationally tunable, and moreover, these “mechanical pixels” can be activated on demand to vary the bulk compres- sive properties. Although PTDs were manually

introduced here, soft robotics-based technology (25), microelectromechanical systems actuator arrays (26), or even thermal fluctuations (27), provide alternative avenues to introduce and remove PTDs. To understand both the density dependence

and compression dependence of the Miura-ori with a PTD, we analytically calculated the in-

trinsic PTD compressive modulus, KPTDy (see sup- plementary materials for details). This was found by noting that the stress a PTD exerts is propor- tional to its extension relative to the neighboring undefected unit cells. At low defect densities for a lattice of arbitrary size, the compressive modulus of a lattice with a PTD can be expressed in a dipole expansion, Kdefecty = K

normal y + nK

PTD y , where K

PTD y

648 8 AUGUST 2014 • VOL 345 ISSUE 6197 sciencemag.org SCIENCE

Fig. 2. Experimental data showing spatial confinement of a PTD and combined experi- mental/theoretical data for PTD mechanics. (A) 3D reconstruction of a Miura-ori with a centrally located PTD (red facets). The color bar is height in mm. (B) Photograph of a single vertex shows that it is mechanically stable in isolation, as is a PTD (C). (D) Mean curvature of 3D scan from (A) shows a modified crease pattern in the presence of a PTD. The color bar is in units of mm–1. Overlapping vertex position of same lattice without a PTD (black dots) shows that the PTD is highly localized and causes minimal distortion in finite-sized lattices. (E) Theoretical energydiagram of a single vertex has two energy minima cor- responding to a (I) normal and (II) PTD state. Arrows indicate direct p

Recommended